Zhang, Yinan (2011) Experimental investigation of the Ca-Mg-Zn system via Diffusion Couples and Key Experiments. Masters thesis, Concordia University.
This is the latest version of this item.
- Accepted Version
Nine diffusion couples and 32 key samples have been used to study the phase diagram of the Ca-Mg-Zn system at 335ºC and crystal structures of ternary intermetallics. Four ternary compounds have been found in this system: Ca3MgxZn15-x (4.6≤x≤12 at 335ºC) (IM1); Ca14.5Mg15.8Zn69.7 (IM2); CaxMgyZnz (x = 8.2-9.1; y = 27.1-31.0; z = 60.8-64.7 at 335ºC) (IM3) and Ca1.5Mg55.3Zn43.2 (IM4). Phase relations and solubility limits have been determined for binary and ternary compounds using Scanning Electron Microscopy, Electron Probe Microanalysis and X-ray Diffraction techniques. Crystal structures of the IM1 and IM3 ternary compounds have been studied by means of XRD, Transmission Electron Microscopy and Electron Back Scattered Diffraction. The refinement of the XRD patterns for IM1 ternary compound has been carried out by Rietveld analysis. XRD data has shown that this solid solution crystallizes in hexagonal structure having P63/mmc (194) space group and Sc3Ni11Si4 prototype. The lattice parameters decrease linearly with decreasing Mg content obeying Vegard’s law. The fractional atomic occupancy of 6h, 4f, 2b and 12k sites of this compound are function of Mg concentration. Focused Ion Beam has been used to lift Transmission Electron Microscopy specimen of the ternary compound and the hexagonal structure has been confirmed by means of Selected Area Electron Diffraction data. Based on the atomic occupancy results and the crystallographic details, a three sublattice (Ca)(Zn)(Mg,Zn)4 model is proposed for this compound.
Three binary compounds are found to have extended solid solubility into the ternary system. CaZn11, CaZn13 and Mg2Ca are forming substitutional solid solutions where Mg substitutes Zn atoms in the first two compounds, and Zn substitutes both Ca and Mg atoms in Mg2Ca. Based on the current experimental results, the isothermal section of Ca-Mg-Zn phase diagram at 335ºC has been constructed. The morphologies of diffusion couples have been studied in the Ca-Mg-Zn system at 335ºC. Depending on the terminal compositions of the diffusion couples, the morphology of the two-phase regions in the diffusion zone has: ‘tooth-like’ morphology or matrix phase with isolated and/or dendritic shape precipitates morphology.
|Divisions:||Concordia University > Faculty of Engineering and Computer Science > Mechanical and Industrial Engineering|
|Item Type:||Thesis (Masters)|
|Degree Name:||M.A. Sc.|
|Date:||10 May 2011|
|Thesis Supervisor(s):||Medraj, Mamoun and Chartrand, Patrice|
|Keywords:||Ca-Mg-Zn; Phase diagrams; Diffusion; Diffraction; Electron microprobe|
|Deposited By:||YI NAN ZHANG|
|Deposited On:||09 Jun 2011 14:37|
|Last Modified:||10 Jun 2011 05:38|
 X. F. Wan, Y. S. Sun, F Xue, J. Bai, W.J. Tao, Microstructure and mechanical properties of AZ62 based magnesium alloys with calcium addition, Transactions of Nonferrous Metals Society of China, Vol. 20, No. 5, 2010, pp. 757-762.
 M. Aljarrah, M. Medraj, X. Wang, E. Essadiqi, G. Dénès and A. Muntasar, Experimental Investigation of the Mg-Al-Ca System, Journal of Alloys and Compounds, Vol. 438, No. 1-2, 2007, pp. 131-141.
 O. Beffort, Ch. Hausmann, The Influence of Ca-additions on the Mechanical Properties of T300-C-Fibre/Mg (Al) Metal Matrix Composites, in: K.U. Kainer (Ed.), Magnesium Alloys and their Applications, 2000, pp. 215–220.
 A.A. Luo, Recent Magnesium Alloys Development for Elevated Temperature Application, International Materials Review, Vol.49, No.1, 2004, pp. 13-30.
 F. Nie and B.C. Muddle, Precipitation Hardening of Mg-Ca (-Zn) Alloys, Scripta Materialia, Vol.37, No.34, 1997, pp. 1475-1481.
 B. Zberg, P. J. Uggowitzer, and J. F. Löffler, MgZnCa Glasses Without Clinically Observable Hydrogen Evolution for Biodegradable Implants, Nature Materials, Published Online: 27th Sep. 2009.
 B. Zberg, E. R. Arataa, P. J. Uggowitzera, and J. F. Löffler, Tensile Properties of Glassy MgZnCa Wires and Reliability Analysis Using Weibull Statistics, Acta Materialia, Vol. 57, No. 11, 2009, pp. 3223-3231.
 U.R. Kattner, The Thermodynamic Modeling of Multicomponent Phase Equilibria, Journal of Metals, Vol. 49, No. 12, 1997, pp. 14-19.
 Y.A. Chang, S. Chen, F. Zhang, X. Yan, F. Xie, R. Schmid-Fetzer and W.A. Oates, Phase Diagram Calculation: Past, Present and Future, Progress in Materials Science, Vol.49, 2004, pp.313-345.
 L. Kaufman and H. Bernstein, “Computer calculation of phase diagrams with special reference to refractory metals”, Academic Press, New York, 1970.
 K.C. Kumar, and P. Wollants, “Some guidelines for thermodynamic optimization of phase diagrams”, Journal of Alloys and Compounds, vol. 320, 2001, pp. 189-198.
 S. Wasiur-Rahman and M. Medraj, Critical assessment and thermodynamic modeling of the binary Mg–Zn, Ca–Zn and ternary Mg–Ca–Zn systems, Intermetallics, Vol. 17, No. 10, 2009, pp. 847-864.
 “FactSage 6.0”, Thermfact (Centre for research in computational thermochemistry), Montreal, QC, Canada, 2010.
 R. Paris, Ternary Alloys, Publications Scientifiques et Techniques du minist’ere de L’Air, Ministère de L’Air, No.45, 1934, pp. 1-86.
 J.B. Clark, The Solid Constitution in the Mg-rich Region of the Mg-Ca-Zn Phase Diagram, Trans. AIME, Vol. 221,1961, pp. 644-645.
 J.B. Clark, Joint Committee on Powder Diffraction Standards (JCPDS) Card 12-0266, 1961.
 J.B. Clark, Joint Committee on Powder Diffraction Standards (JCPDS) Card 12-0569, 1961.
 T.V. Larinova, W.W. Park, and B.S. You, A Ternary Phase Observed in Rapid Solidified Mg-Ca-Zn alloys, Scripta Materialia, Vol. 45, 2001, pp. 7-12.
 P.M. Jardim, G. Solorzano, and J.B.V. Sande, Precipitate Crystal Structure Determination in Melt Spun Mg-1.5wt%Ca-6wt%Zn Alloy, Mircoscopy and Microanaysis, Vol. 8, 2002, pp. 487-496.
 P.M. Jardim, G. Solorzano, and J.B.V. Sande, Second Phase Formation in Melt-spun Mg-Ca-Zn Alloys, Materials Science and Engineering A, Vol. 381, No. 1-2, 2004, pp. 196-205.
 K. Oh-ishia, R. Watanabeb, C.L. Mendisa, and K. Hono, Age Hardening Response of Mg-0.3 at.% Ca alloys with different Zn contents, Materials Science and Engineering: A, Vol. 526, No. 1-2, 2009, pp. 177-184.
 C. O. Brubaker and Zi-Kui Liu, A computational thermodynamic model of the Ca–Mg–Zn system, Journal of Alloys and Compounds, Vol. 370, No. 1-2, 2004, pp. 114-122.
 J. S. Kirkaldy and L.C. Brown, Diffusion Behaviour in the Ternary, Multiphase Systems, Canadian Metallurgical Quarterly, Vol. 2, No. 1, 1963, pp. 90-115.
 J. B. Clark, Conventions for Plotting the Diffusion Paths in Multiphase Ternary Diffusion Couples on the Isothermal Section of a Ternary Phase Diagram, Transactions of the Metallurgical Society of AIME, Vol. 227, 1963, pp. 1250-1251.
 A.A. Kodentsov, G.F. Bastin, and F.J.J. van Loo, The Diffusion Couple Technique in Phase Diagram Determination, Journal of Alloys and Compounds, Vol. 320, No. 2, 2001, pp. 207-217.
 J.C. Zhao, A Combinatorial Approach for Structural Materials, Advanced Engineering Materials, Vol. 3, No. 3, 2001, pp. 143-147.
 J.C. Zhao, A Combinatorial Approach for Efficient Mapping of Phase Diagram and Properties, Journal of Materials Research Society, Vol. 16, No. 6, 2001, pp. 1565-1578.
 J.C. Zhao, M. R. Jackson, and L.A. Peluso, Determination of the Nb-Cr-Si Phase Diagram Using Diffusion Multiples, Acta Materialia, Vol. 51, No. 20, 2003, pp. 6395-6405.
 H.H. Xu, Y. Du, Y.C. Zhou, and Z.P. Jin, Determination of Phase Diagram Using the Diffusion Couple Technique, Rare Metals, Vol. 25, No. 5, 2006, pp.427-430.
 H. Putz, K. Brandenburg, Pearson’s Crystal Data, Crystal Structure Database for Inorganic Compounds, CD-ROM software version 1.3.
 A.J. Schwartz, M. Kumar, B.L. Adams, Electron Backscatter Diffraction in Materials Science, Kluwer Academic/Plenum Publishers, Dordrecht/New York, 2000.
 J.J. Park and L.L.Wyman, Phase Relationships in Magnesium Alloys, WADC Tech. Rept. 57-504, Astia Document No. AD142110, 1957, pp. 1-27.
 F.J.J. van Loo and G.D. Rieck, Diffusion in the titanium-aluminium system—I. Interdiffusion between solid Al and Ti or Ti-Al alloys, Acta Metallurgica, Vol. 21, No. 1, 1973, pp. 61-71.
 F.J.J. van Loo and G.D. Rieck, Diffusion in the titanium-aluminium system—II. Interdiffusion in the composition range between 25 and 100 at.% Ti, Acta Metallurgica, Vol. 21, No. 1, 1973, pp. 73-84.
 B.Y. Kotur, M. Sikiritsa, O.I. Bodak, E.I. Gladyshevskii, Crystal structure of the compound Sc3Ni11Si4, Sov. Phys. Crystallogr. Vol. 28, 1983, pp. 387-389.
 A.R. Denton and N.W. Ashcroft, Vegard’s Law, The American Physical Society, Vol. 43, No. 6, 1991, pp. 3161-3164.
 D.W. Deng, K.H. Kuo, Z.P. Luo, D.J. Miller, M.J. Kramer and K.W. Dennis, Crystal structure of the hexagonal Zn3MgY phase, Journal of Alloys and Compounds, Vol. 373, No, 1-2, 2004, pp. 156-160.
 W.D. Callister, Materials Science and Engineering: An Introduction, John Wiley & Sons, Inc, 2003.
 M. Latroche, P. Kalisvaart and P.H.L. Notten, Crystal structure of Mg0.65Sc0.35Dx deuterides studied by X-ray and neutron powder diffraction, Journal of Solid State Chemistry, Vol. 179, No. 10, 2006, pp. 3024-3032.
Available Versions of this Item
- Experimental investigation of the Ca-Mg-Zn system via Diffusion Couples and Key Experiments. (deposited 09 Jun 2011 14:37) [Currently Displayed]
Repository Staff Only: item control page